The Effect on the Flexural Strength, Flexural Modulus and Compressive Strength of Fibre Reinforced Acrylic with That of Plain Unfilled Acrylic Resin – An in Vitro Study
Tony C Thomas1, Aswini Kumar K2, Shamaz Mohamed3, Vinod Krishnan4, Anil Mathew5, Manju V6
ABSTRACT Aim: The aim of this in vitro study was to compare the flexural strength, the flexural modulus and compressive strength of the acrylic polymer reinforced with glass, carbon, polyethylene and Kevlar fibres with that of plain unfilled resin. Materials and Methods: A total of 50 specimens were prepared and divided into 10 specimens each under 5 groups namely group 1- control group without any fibres, group 2 – carbon fibres, group 3- glass fibres, group 4 – polyethylene, group 5- Kevlar. Universal testing machine (Tinius olsen, USA) was used for the testing of these specimens. Out of each group, 5 specimens were randomly selected and testing was done for flexural strength using a three point deflection test and three point bending test for compressive
strength and the modulus was plotted using a graphical method. Statistical analysis was done using statistical software. Results: The respective mean values for samples in regard to their flexural strength for PMMA plain, PMMA+ glass fibre, PMMA+ carbon, PMMA+ polyethylene and PMMA+ Kevlar were 90.64, 100.79, 102.58, 94.13 and 96.43 respectively. Scheffes post hoc test clearly indicated that only mean flexural strength values of PMMA + Carbon, has the highest mean value. One-way ANOVA revealed a non-significant difference among the groups in regard to their compressive strength. Conclusion: The study concludes that carbon fibre reinforced samples has the greatest flexural strength and greatest flexural modulus, however the compressive strength remains unchanged.
Keywords: Glass, Kevlar fibres, Polyethylene, Poly methyl methacrylate
MATERIALs AND METHODs
The introduction of poly methyl methacrylate (PMMA) in 1937 by Dr. Walter Wright, heralded a new age in the field of prosthodontics . The PMMA was so well received by the dental profession, that currently most of the dentures are constructed by this. The ease of use, biocompatibility, excellent aesthetics and ease of repair makes this, the material of choice for denture bases. The PMMA have a wide variety of application not only as a denture base material but also as a denture repair material, material for artificial teeth, record base, facing for crowns and bridges, special trays, material for making obturator, etc. The desirable qualities of PMMA is offset by certain drawbacks, significant among them are its reduced strength and stiffness. Various researchers have proposed modalities for strengthening the resin like- embedding of solid metal forms in the resin, incorporation of a rubber phase in the bead polymer, reinforcing of acrylic resin with various fibres [2-4].
A total of 50 specimens were prepared and divided into 10 specimens each under 5 groups, which were divided according to the reinforcement material used. The specimens for testing the flexural strength, the flexural modulus and compressive strength were fabricated using stainless steel dies. The dimensions of each test specimen were length 60mm x width 10mm x thickness 4mm. The dies were invested in number 7 varsity flask (Jabbar & co, Aligarh, India) using type III Gypsum (Goldstone, Asian chemicals, India). Once the dental stone was set, the two halves of the flask were separated and the dies were lifted out of the mould. Sodium alginate separating medium (DPI, India) was applied on the mould [Table/Fig-1]. The packing of PMMA (DPI- Dental product of India) was done during dough stage. Initially a thin layer of acrylic material was evenly spread over the mould space. The fibre specimens were prepared by cutting the fibre slightly short of the length of acrylic specimens and weighed. The pre weighed amount of fibres (5% by weight of acrylic) depending on the group (group 2 – carbon fibres, group 3- glass fibres, group 4 – polyethylene, group 5- Kevlar, All fibres manufactured by VSSC-Vikram Sarabhai, Space Research Centre, India) were spread over this thin layer of acrylic. Care was taken to prevent over extension of the fibres outside the mould space. Another layer of acrylic was placed over the fibres. Trial packing was done and manufactures instructions were followed during the process of curing and finishing. Group 1 was kept as a control group without any fibres incorporated. All the specimens were stored in water at room temperature before testing. Universal testing machine (Tinius olsen, USA) was used for the testing of specimens.
The embedding of solid metal forms resulted in poor aesthetics [2,5] whereas the incorporating of rubber phase [6-8] in the bead polymer worked out to be expensive. These limited the use of fibres to reinforce the acrylic. Various studies reveal a significant increase in physical and mechanical properties of reinforced acrylic resin. The commonly used fibres to strengthen acrylic resin are carbon [9-12] glass [2,5,13] polyethylene [14-20] and Kevlar [7,21] However, there is paucity of information in literature on the comparison of all the above fibres with regard to their mechanical properties. The aim of this in vitro study was to compare the flexural strength, the flexural modulus and compressive strength of acrylic polymer reinforced with glass, carbon, polyethylene and Kevlar fibres with that of plain unfilled resin. 12
Journal of Clinical and Diagnostic Research. 2015 Mar, Vol-9(3): ZC12-ZC14
Tony C Thomas et al., The Effect on the Flexural Strength, Flexural Modulus and Compressive Strength of Fibre Reinforced Acrylic
Out of each group 5 specimens were randomly selected and testing was done for flexural strength using a three point deflection test with a cross head speed of 3mm/min. The parallel arms of the jig were kept 50 mm apart. The specimen is positioned on the jig and load was applied on the centre as shown in the [Table/Fig-2].
were 2.55, 2.69, 3.06, 2.42 and 2.78 respectively. One-way ANOVA revealed a significant difference (p